1 Cavendish Laboratory, Department of Physics, University of Cambridge, J. J. .... Light-induced (right) and dark-state (left) crystal structures of 1 at 100 K, ...
Aug 15, 2001 - Macroscopic Heterogeneities in Electroosmotic and Pressure-Driven Flow through Fixed Beds at Low Column-to-Particle Diameter Ratio.
MoisturePeeling of House Paints. Mechanism of. Moisture. Peeling. J. W. ILIFF AND R. R. DAVIS. E. I. du Pont de Nemours and Company,Inc., Philadelphia, ...
Moisture Peeling of House Paints Mechanism of Moisture Peeling. J. W. Iliff, and R. B. Davis. Ind. Eng. Chem. , 1939, 31 (12), pp 1446â1450. DOI: 10.1021/ ...
arrangement similar to the structure of ice. (J Phys Chem B .998 102 569-76). SCIENCE. Peeling oligosaccharides. Sequencing oligosaccharides can be tricky.
Citation data is made available by participants in Crossref's Cited-by Linking service. For a more comprehensive list of citations to this article, users are ...
Oct 10, 2017 - Compared with conventional graphene, few-layer graphene is an easy-to-use material because of its interesting mechanical and chemical properties. Meanwhile, solution plasma (SP) represents a nonequilibrium discharge, which induces elec
Sangwoo Chaea, Maria Antoaneta Bratescua, and Nagahiro Saitoa,b* .... band dispersion near the Fermi level in few-layer graphene does not strongly depend ...
Moisture Peeling of House Paints. Mechanism of. Moisture Peeling. J. W. ILIFF AND R. a. DAVIS. E. 1. du Pont de Nemours and Company, Inc., Philadelphia, ...
Subscriber access provided by ALBRIGHT COLLEGE
Light-Induced Macroscopic Peeling of Single-Crystal Driven by Photoisomeric Nano-Optical Switching Jacqueline M. Cole, Jose de J. Velazquez-Garcia, David J Gosztola, SuYin Grass Wang, and Yu-Sheng Chen Chem. Mater., Just Accepted Manuscript • DOI: 10.1021/acs.chemmater.9b01738 • Publication Date (Web): 11 Jun 2019 Downloaded from http://pubs.acs.org on June 11, 2019
Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.
Light-Induced Macroscopic Peeling of SingleCrystal Driven by Photoisomeric Nano-Optical Switching Jacqueline M. Cole,1,2,3,4,* Jose de J. Velazquez-Garcia,1 David J. Gosztola,4 SuYin Grass Wang5, Yu-Sheng Chen5 1
Cavendish Laboratory, Department of Physics, University of Cambridge, J. J. Thomson Avenue, Cambridge, CB3 0HE, UK
ISIS Neutron and Muon Source, STFC Rutherford Appleton Laboratory, Harwell Science and Innovation Campus, Didcot, Oxfordshire, OX11 0QX, UK 3
Department of Chemical Engineering and Biotechnology, University of Cambridge, West Cambridge Site, Philippa Fawcett Drive, Cambridge, CB3 0AS, UK 4
Argonne National Laboratory, 9700 S. Cass Avenue, Lemont, IL 60439, United States
NSF’s ChemMatCARS Beamline, The University of Chicago, Advanced Photon Source, Lemont, IL 60439, United States
Single-crystal optical actuators are emerging as a prospective material form for nano-optical mechanical switching, sensing or transduction device applications in nanotechnology and quantum technology. Crystal-lattice strain effects lie at the molecular origins of their macroscopic optical behaviour, and linkage photo-isomerization is an attractive source of optical actuation if only suitably functioning materials of this ilk could be found. We discover ƞ1-SO2 to ƞ1-OSO
phenylpyridine)]Cl2·H2O which behaves macroscopically as an single-crystal optical actuator, whereby the crystal peels in response to light-induction at 100 K. It thermally recovers, whereupon the crystal exhibits remarkable restorative properties. We apply photocrystallography alongside concerted optical microscopy and optical absorption spectroscopy to reveal how the molecular origins of photo-isomerization induce crystal-lattice strain that engenders this macroscopic crystal peeling effect. Linking structure and function across molecular and macroscopic length scales showcases a means by which single-crystal optically actuating materials could be systematically designed.
Crystals have been long been held as rigid and static forms of materials, owing to their highly regularized and periodic lattice frameworks of ordered molecules. Out-of-equilibrium phenomena can nonetheless exist within the crystalline state when they are driven by an external stimulus. Such phenomena often engender the function of a material, while the ordered nature of single crystals offers high consistency in fabrication if they could operate as actual devices. Learning how to control out-of-equilibrium phenomena within single crystals that can act as devices thus presents an enormous opportunity for functional materials science. Single-crystal optical actuators are emerging as candidates for key applications in nanotechnology1,2 and quantum-technology,3 owing to their function as nano-optical switches, sensors or transducers, especially where they can be used to create a macroscopic mechanical motion.
Single-crystal optical actuators are being found that display a variety of macroscopic responses to light-stimuli:4 bending, twisting, coiling, jumping, creeping, and exploding. These are all forms of elastic or plastic deformation. Most of these actuators discovered to date are the result of photo-induced chemical reactions that can occur within single-crystals; the chemical product is realized via a light-induced structural transformation within the crystal lattice, building up strain that is typically alleviated by a mechanical response.5-12 While some of these reactions are reversible, the strain induced causes many crystals to explode. Moreover, most of these case studies are organic materials, whose limited thermal stability has presented major historical issues for practical applications in the wider field of photonics.13 Metal-organic complexes offer
much better thermal stability while retaining their organic versatility. Certain metal-organic complexes can exhibit linkage photo-isomerism which operates via a nano-optical switching mechanism.14 This could provide a route to single-crystal optical actuation. Additionally, its intramolecular origins make it particularly attractive to device technology: for example, it is more controllable and requires less energy than intermolecular reactions. That said, the material, [Co(NH3)5(NO2)]Cl(NO3), appears to stand alone in reports that demonstrate both single-crystal linkage photo-isomerism15 and single-crystal optical actuation.16 While these reports acknowledge that crystal-lattice strain at the molecular level must govern their macroscopically observed optical actuation, they state that its molecular characterization was compromised heavily by the tendency of its crystals to fracture.
In this study, we showcase the discovery of a new single-crystal optical actuator, [Ru(NH3)4(SO2)(3-phenylpyridine)]Cl2H2O (1), whose mechanism is governed by single-crystal linkage photoisomerism. Crucially, we enable an intrinsic link between its macroscopically observed optical phenomenon and its molecular origins by coupling concerted optical microscopy and absorption spectroscopy with a light-induced in situ single-crystal X-ray diffraction study. Creating this link is incredibly important, since it lays a foundation for a systematic approach to the molecular design of single-crystal optical actuators. The dark and light-induced crystal structures of 1 were captured using in situ photo-stimulated single-crystal X-ray diffraction at 100 K. These structures reveal the nano-optical switching, which is caused by ƞ1-SO2 to ƞ1-OSO linkage photo-isomerization. We then demonstrate how this light-induced structural change results in the macroscopic peeling of a single crystal of 1 at 100 K, using a custom-built concerted optical absorption microscopy and spectroscopy set-up with N2 cryogenic
capabilities. We observe that this crystal peeling effect is thermally reversible to the extent that it shows remarkable restorative properties upon warming to room temperature. Pseudo-merehedral twinning appears to be crucial to this light-induced macroscopic crystal motion, whose mechanism tracks a five-step process: (i) SO2 linkage photo-isomerization, which (ii) builds up crystal-lattice strain, which (iii) is alleviated by crystal buckling, which (iv) enables further optical absorption and photo-isomerization which, in turn, (v) yields a compensatory curling effect.
Results and Discussion
The solid-state ƞ1-SO2 to ƞ1-OSO linkage photo-isomerization that affords the single-crystal nano-optical switching phenomenon in 1 is illustrated in Figure 1. The most thermally stable Sbound ƞ1-SO2 ligand configuration (Figure 1, top left) is generally expected for SO2 ligand coordination, as is represented by our dark-state crystal structure determination of 1 (Figure 1, bottom left). These crystallographic data were obtained from a 120 x 30 x 5 µm3 crystal, held at 100 K, using synchrotron-based single-crystal X-ray diffraction at the NSF’s ChemMatCars beam line of the Advanced Photon Source, USA. The light-induced crystal structure of 1 (Figure 1, right) was then deduced by applying green light ( = 505 nm) to this crystal for 2.5 hours, while holding its diffractometer position and temperature at 100 K, and then acquiring and processing an otherwise identical data set. Details of this developing in situ light-stimulated single-crystal X-ray diffraction method, becoming known as photo-crystallography, are described elsewhere17-20 and in the Supporting Information. 52(3)% of the SO2 ligands in the crystal lattice of 1 were found to photo-convert to an O-bound ƞ1-OSO configuration, as
indicated by the hollow-bonded SO2 ligand coordinated to ruthenium in light-induced crystal structure of 1 (Figure 1, bottom right). Its residual 48(3)% dark-state SO2 component (solidbonded SO2 ligand shown in Figure 1, bottom right) is tilted slightly to accommodate this linkage photo-isomerism.
Figure 1. (top) Schematic of the linkage photo-isomerization process observed in 1. (bottom) Light-induced (right) and dark-state (left) crystal structures of 1 at 100 K, showing anisotropic displacement parameters at the 50% probability level. The ƞ1-OSO photo-isomer is shown with hollow-bonds, while the ƞ1-SO2 ligand configuration is presented with solid-bonds. Hydrogen atoms, chloride ions and the water of crystallization are omitted for clarity.
In common with other nano-optical switching ruthenium-based sulfur dioxide ammine (hereafter denoted [Ru-SO2]) complexes,21-29 this light-induced structure of 1 exists as a metastable state at 100 K, and reverts to its dark-state crystal structure once warmed to room temperature. However, the nano-optical switching of 1 is distinctly untypical for this family of ruthenium-based complexes, in that it only presents with the ƞ1-OSO photo-isomer; all other reports on [Ru-SO2] complexes manifest a S-O side-bound ƞ2-SO2 type of photoisomerization21,22,24 or a mix of that with some ƞ1-OSO photo-isomerization.23,25-29 Moreover, the 52(3)% ƞ1-OSO photo-conversion fraction in 1 is the highest observed in all [Ru-SO2] complexes reported to date. This stands to reason considering both steric and chemical characteristics of the 3-phenylpyridine trans ligand in 1. 3-phenylpyridine affords the largest steric contribution of any 3-substituted pyridine trans ligand in photocrystallographically reported [Ru(SO2)] complexes. In terms of chemical properties, the nitrogen atom in 3phenylpyridine possesses the second largest pKa value (4.73)
of any 3-substituted pyridine
ligand in these [Ru(SO2)] structures. The largest pKa value of a trans ligand in reported [Ru(SO2)] crystal structures belongs to 3-pyridine (pKa = 5.12),30 whose [Ru(SO2)(NH3)4(3pyridine)]Cl2.H2O photocrystallographic structural counterpart to 1 displayed the largest ƞ1-OSO photo-conversion fraction (44.5(7) %) until now,29 given the report herein on 1 with 52(3) %.
1 crystallizes as a pseudo-merehedral twin, where librational disorder of the phenyl group in its 3-phenylpyridine ligand confines the space-group symmetry to P21 (see Supporting Information). The unit cell dimensions of 1 change substantially upon photo-conversion, whereby all unit cell lengths change by ~1% while changes by 2% (see Supporting Information, Table S4). subtends the a,c-crystallographic plane, in which all of the bond-geometry changes of the SO2
photo-isomerization effect occur (see Supporting Information, Figure S1). The unit cell length that changes most upon photo-conversion is c, to which the ƞ1-Sbound-Ru-Npyridyl axis is primarily aligned; this axis hosts the largest light-induced bond-length changes in 1, with Ru1-N5 (dark) 2.119(4) Å; Ru1-N5 (light) 2.062(8) Å; i.e. (Ru-Npyridyl) = 1.3 %, and Ru1-S1 2.1173(14) Å; Ru1-S1 (light) 2.22(2) Å; i.e. (Sbound-Ru) = 4.9 % (see Supporting Information, Table S5, for more details about light-induced changes in the Ru-coordination geometry). The fact that these particularly large bond-geometry changes occur along this S-Ru-N axis stand to reason, considering the substantial trans influence that is expected to manifest in 1 owing to the large pKa value of 3-phenylpyridine which, in turn, explains the large SO2 photo-conversion fraction.26,29
The macroscopic manifestation of this nano-optical switching phenomenon in single-crystals of 1 was studied via low-temperature optical microscopy. This apparatus formed part of a custom-built concerted optical microscopy and absorption spectroscopy set up with an optics bench to deliver controlled incident green light to a single-crystal that was housed inside an optical cryostat with temperature control. Further details are given in Supporting Information, as are full movies of the various optical microscopy time sequences discussed below, while only selected frames are presented in Figures 2 and 3.
Figure 2 (top panel) shows how a single-crystal of 1 responds to t minutes of stimulation by green ( = 505 nm) light while held at 100 K. The time-sequence shows a remarkable crystal ‘peeling’ effect that begins with the light-induced lateral cut in the crystal seen at the t = 20 min snapshot, and spans through to t = 1600 min during which a crystal segment on one side of this
cut progressively curls as it continues to be exposed to more light. A progressive darkening of the crystal is associated with this light-induced effect. Such photochromic changes are commonly observed in [Ru-SO2] complexes, while this macroscopic crystal ‘peeling’ effect is unprecedented. Dark lines can be seen in the lateral sections inside the cut at the higher time regimes, e.g. there are two intensely dark lateral lines inside the cut at t = 1600 min, at the time when the peeling has finally extended as far as it can.
This light-induced structural effect in 1 was then reversed by warming the crystal to room temperature. Figure 2 (bottom panel) shows that the crystal reverts to its original color within 70 K, as is fairly typical for the thermal decay of an ƞ1-OSO photoisomer in [Ru-SO2] complexes; the exact decay lifetime depends on the warming rate which, in our case was 1.5 K / 5 sec within the 100-200 K temperature elevation stage. The photochromic (and thus photo-isomeric) reversion occurs before the crystal peeling effect has subsided. The increase in transparency of the crystal reveals that the light-induced cut is actually caused by a buckling effect, cf. the raised crystal sections either side of the cut, which gradually close in synchrony much like the operation of a two-sided drawbridge. This closure occurs as a function of increasing temperature, but primarily during 230-250 K, which corresponds precisely to the temperature range in which a heavy drop in viscosity is observed for the perfluoroether oil that holds the crystal frozen on a sapphire disk within the optical cryostat. Thus, a physical ‘clamping’ effect is apparent, and seems to trap this macroscopic crystal peeling phenomenon, long after the photoisomer has decayed; this finding bears striking parallels to crystal clamping effects observed in many types of phase transitions and mode softening phenomena.31-33 Notice that the cut does not fully close
and the lines from the ‘drawbridge hinges’ remain in the crystal, even after it reaches room temperature.
Figure 2. (top panel) Eight optical microscopy snapshots of a movie that illustrates the crystal peeling as a response to t minutes of its first cycle of light induction (λ = 505 nm) at T = 100 K. A photochromic change from orange to deep blue is shown which is caused by an associated linkage photo-isomerization effect (bottom panel) Eight optical microscopy snapshots of a movie that demonstrates the partial thermal recovery of the crystal whereby the peeling is largely reversed as the crystal is warmed to temperature, T. A crystal buckling effect that initiated this crystal peeling effect is apparent in these images. See Movie S1 for further illustration.
Figure 3 (top panel) demonstrates quite remarkably that the cut can nonetheless be fully closed by repeating the light-induction (albeit for only 30 min) and warming cycle. The corresponding time sequence upon warming reproduces the same trend that was tracked in Figure 2 in that the drawbridge closes primarily between 230-250 K, but with the stark exception that the cut closes much more tightly, such that the two sides of the drawbridge are seen to touch in the panel marked with T = 246 K. The next panel (T = 249 K) shows that the right-hand drawbridge hinge has disappeared, and a thick dark line rests in place of the cut. This dark line moves closer to the left-hand hinge line upon warming to T = 271 K, and appears much thinner.
Figure 3 (bottom panel) presents a third cycle of inducing light and warming the crystal. Four time snapshots that span 90 minutes of light induction first reveal that while the dark line that resides from the cut location becomes thicker, it does not re-open. Rather, a series of other dark lines form laterally across the crystal, perhaps best seen at the t = 37 min snapshot before the crystal becomes as dark as it can be by only 90 min of light induction, judging from the darkness achieved by the other light-induced cycles. The line pertaining to the original cut location is no thicker than many of these lines, indicating that it is no more vulnerable than some of the other lines in being the point of crystal buckling. In other words, the crystal appears to have sufficiently restored its crystal forces within this domain line that it has essentially healed itself. The third cycle of crystal warming (Figure 3, bottom row) suggests that these many lateral lines all result from the same type of light-induced crystal-lattice strain that was previously alleviated by the crystal peeling effect, by virtue of the fact that these lines dissipate in the same temperature region where the crystal stops being frozen to its substrate (240-250 K).
Figure 3. (top panel) Eight optical microscopy snapshots of a movie that illustrates the warming effect during a second cycle of light-induction (albeit for only t = 30 min) followed by heating to room temperature. The images show how the crystal peeling effect fully recovers upon warming as the crystal cut closes completely. (bottom panel) Two pairs of four optical microscopy snapshots of a movie which illustrate respectively the first and second parts of a third cycle of crystal light-induction (albeit for only t = 90 min) followed by warming to room temperature. These time sequences show how the crystal has restored itself to the extent that its residual domain line does not reopen upon application of light; instead, other domain lines form to accommodate the light-induced crystal strain. The domain line residing from the crystal restorative process appears to be no more susceptible than the other domain lines toward crystal buckling. See Movie S2 and Movie S3 for further illustration of cycles 2 and 3, respectively.
Simultaneous optical absorption spectroscopy was performed alongside these optical microscopy studies, since photo-isomerization changes can be inferred indirectly from various modulations in metal-ligand charge-transfer (MLCT) that manifest as changes in optical absorption. While our single-crystal X-ray diffraction studies have provided a 3-D representation and quantitative measure of photo-isomerization, photo-crystallography is a bulk technique; it therefore becomes of limited use once a crystal begins to peel. In contrast, optical absorption spectroscopy can measure time sequences of optical absorption at highly localized points in a crystal. This is very poignant to this study where we wish to understand the correlated structural and optical absorption changes inside and outside of the cut observed in the crystal, where there exists a distinct optical absorption gradient. Indeed, the optical microscopy shows that the crystal is more transparent inside the cut, relative to that of its exterior surface, as we saw in Figure 2. The exposure of the crystal interior engendered by this cut thus allows light to penetrate deeper into the crystal such that it absorbs more light. Light must nonetheless pass through the entire crystal; otherwise the crystal would not be observed by optical microscopy or spectroscopy as it operates in transmission mode.
Accordingly, the optical absorption spectra shown in Figure 4 were collected on the crystal at two locations: one outside the cut and one inside the cut, as indicated by the white circles in the crystal overlays. These spectra relay the time series of optical absorption changes that occur during the first cycle of light-induction, which were measured in tandem with the optical microscopy images shown in Figure 2. Note that the crystal suddenly absorbs more red light at t = 20 mins, which quickly dissipates at both crystal locations shown; this is presumably caused by the newly exposed surface inside the cut adjusting to a change in optical absorption with
respect to the deeper interior of the crystal. The optical absorption of the crystal at both locations then recovers and thereafter increases monotonically, while their respective overarching spectral profiles remain essentially constant. By t = 80 mins, the absorption has plateaued, rendering the crystal region outside the cut as a black body for visible light, while the region inside the cut retains a dip in optical absorption between 500-600 nm, affording it a deep blue hue. The optical densities inside and outside of the cut remain different throughout this time sequence, as is expected given the thinner crystal cross-section associated with the measurements within the cut.
This difference in optical density will induce a particularly acute absorption contrast at the point of the crystal buckling hinge; indeed, careful observation of this region in Figure 2 (top panel) reveals a bright line that tracks the intersection of the right-hand hinge with the inside of the cut, as the hinge moves along the crystal face. There will presumably be a commensurate photo-isomerization contrast in the region of this hinge. Since an increase in optical absorption tends to be correlated with an increase in levels of photo-isomerization, the hinge will likely open up to alleviate the light-induced crystal strain caused by this contrast. The hinge opens up via a curling effect that lessens with increasing light-induction, becoming barely discernible above t = 80 mins where the optical absorption has plateaued.
Figure 4. (a) Single-crystal optical absorption spectra of 1 at 100 K acquired during the first cycle of the light-induction process in concert with the optical microscopy images illustrated in Figure 2. The optical microscopy overlay in each spectrum carries a white circle that pinpoints the location on the crystal that the optical absorption spectrum probed. i.e. (a) outside and (b) inside the light-induced crystal cut. (c) The unit cell parameters of the dark- and light-induced crystal structure of 1. (d, inset) The orientation of the crystal with respect to these unit cell parameters. (d) The five-step mechanism by which a pseudo-merehedral twinned crystal of 1 undergoes (i) ƞ1-SO2 to ƞ1-OSO linkage photoisomerization whose changes in unit cell parameters present the buildup of (ii) light-induced crystal strain which results in a (iii) crystal buckling effect to alleviate this strain, which affords a cut in the crystal surface into which (iv) more light absorbs which enables more linkage photo-isomerization which in turn produces a compensatory (v) crystal curling effect. The overall mechanism represents a macroscopic crystal peeling effect, which is nonetheless linked to its nano-optical switching origins at the molecular scale.
We now propose a five-step mechanism that relates the nano-optical switching effect to the observed macroscopic crystal peeling behavior. Figure 4 (boxed image, middle left) shows how the crystal habit of the sample displayed in Figures 2 and 3 is oriented with respect to its crystallographic axes; the ability to map the axes associated with these nano-scopic and macroscopic effects is a pre-requisite to uncovering the peeling mechanism. The twinned nature of the crystal obscures a precise determination of the Miller index associated with its large crystal face, although it was judged to be close, if not identical, to a (001) plane. Figure 4 (bottom half) shows that the pseudo-merehedral twinning of 1 is a necessary starting point for this mechanism, given that it requires crystal domains which differ by a reversal of the crystallographic b-axis. The ± b variation that results from the pseudo-merehedral twinning of 1 thus engenders twin boundaries that align with the photo-induced domain lines observed laterally across the crystal.
The external light (λ = 505 nm) associated with the photo-isomerization (Figure 4, step (i)) lies incident to the normal of the large crystal face, which undergoes optical absorption at 100 K. Given our earlier note that the photo-crystallographic structure of 1 features SO2 photoisomerization contained within the a,c-crystallographic plane and that the largest bond-geometry changes are directed along c, this external green light will pass along the direction of maximum light-induced structural change. Accordingly, light-induced crystal-lattice strain builds up in the crystal as it progressively absorbs this green light and thus engenders more SO2 photo-isomers. The anisotropic nature of this strain can be inferred by the cell parameters of the dark- and lightinduced crystal structures (Figure 4, top right). These show that the SO2 linkage photoisomerization causes the b- and c-crystallographic planes to expand and the angle between the
a,c-plane (β) to extend, while the crystallographic a-axis contracts. These changes and associated forces are depicted in step (ii) of Figure 4.
The photo-crystallographic results showed that the percentage change in β observed upon photo-stimulation is about double that of any of the unit cell axes (cf. 1% changes in a, b or c versus a 2% change in β). The competing effects of the contracting a-axis against the expansion of all of the other cell parameters cause the crystal to buckle between the b,c-planes. The twin boundaries that lie along b present natural weak domain walls to enable this crystal buckling process; this is represented by step (iii) of Figure 4. The cut in the crystal created by this buckling effect permits more light to penetrate deeper into the crystal. This increases its optical absorption and thence photo-isomerization levels (Figure 4, step (iv)), as indicated by the optical spectra (Figure 4, top) whose absorption continues to change until about 80 min of light induction. An absorption contrast builds up between the two crystal surfaces that are exposed to the light, wherein the hinge of the crystal buckling effect is particularly susceptible to the associated light-induced crystal strain. The hinge opens up in response via a curling action (Figure 4, step (v)).
The observation that this motion response is a curling effect, rather than another type of macroscopic response, appears to be a result of various nano-scopic origins. It is no coincidence that β involves a rotation whose unique crystallographic b-axis lies precisely along the axis of the curling motion observed. The crystal symmetry of 1 is also relevant in that β relates to commensurate changes in the a,c-crystallographic plane, in which the SO2 photoisomerization effects are contained; a corollary is that the curling behavior effectively accommodates the
spatial changes caused by SO2 photo-isomerization effects. The peeling phenomenon will also act in response to the largest bond-changes in 1 that are associated with the SO2 photoisomerization effect; these concern the significant geometric perturbation in Ru-coordination, along its S-Ru-N axis, which aligns close to the direction of the crystallographic axis, c, i.e. normal to the crystal face that peels. Presumably, this curling effect will also alleviate the librational disorder of the 3-phenylpyridine that engenders motion in this peeling direction (see Supplementary Information, Figure S1).
Eventually, light-induced crystal strain appears to impose a limit on the extent of curling, judging from the Movies in the Supplementary Information, which indicate a progressive halting of the peeling effect, as the strain lines increase in strength and number. Once a sufficient amount of crystal strain has built up, no amount of additional incident light will force the crystal to peel further, as was shown earlier in Figure 2, whereby peeling barely extended beyond 300 min of light-induction and by t = 1600 min the crystal was entirely stationary. Thus, the ƞ1-OSO photo-conversion fraction in 1 would appear to have an upper bound. Overall, this series of forces and motions afford the macroscopic crystal peeling effect observed.
The crystal appears to return to its original state via the reverse procedure with a few exceptions: The external stimulus is heat rather than light. Its optical absorption drops quickly with rising temperature, as the O-bound ƞ1-OSO photo-isomer reverts to its more thermally stable S-bound ƞ1-SO2 dark-state ligand configuration. The peeling effect (buckling and curling) remains long after the photo-isomer has disappeared, owing to the aforementioned clamping effects; these render a substantial level of residual strain in the crystal, until the oil used to freeze
the crystal on the substrate within the optical cryostat melts. The crystal buckling does not reverse until a second cycle of light- and heat-induction, whereupon the two sides of its ‘drawbridge’ become sufficiently close that the crystal lattice can reform. The restorative effect of this crystal provides key insights into the mechanistic forces that govern its molecular origins. In particular, it suggests that the crystal lattice forces are sufficiently strong that they pull the crystal together, to the extent that crystal region associated with the original light-induced cut is no weaker than the rest of the crystal upon a third cycle of light induction, cf. many strain lines build up in cycle 3 of light-induction but the crystal is not cut by light (see SI Movie 3). The restorative nature of these photo-induced crystal actuators bears strong parallels to restorative effects that have been observed in thermally- and mechanically-stimulated crystals.34-36
Tests for reproducibility were also performed, whereby a second crystal of 1 was photo-excited with λ = 505 nm at 100 K, and monitored by optical microscopy over three cycles of lightinduction and warming. The optical microscopy employed the same experimental set up as for the first crystal, except that a 20 x objective (0.40 NA, Olympus, UMPLlanF1) was used for cycles 2 and 3 for this second crystal, whose starting dimensions were 0.350 x 0.050 x 0.010 mm3. The peeling effect was reproduced in this second crystal through all three cycles of investigation, as illustrated via Movies S4-S6 in the Supplementary Information. The peeling effect in this crystal emanates from one end of the crystal which, together with its extended length, facilitates a clear visualization of the associated light-induced crystal strain lines; these manifest as dark lateral lines on the main crystal face or as actual optical cuts through the crystal, and appear to form step-wise along the crystal as they increase in number, in response to more and more light being applied to the crystal. The much larger aspect ratio of the second crystal
(35:5 = 7.00) compared to the main subject crystal (19:7 = 2.71) enables the formation of a much longer chain of strain lines that act to progressively temper and eventually halt the crystal peeling effect. Thus, it stands to reason that the peeling effect in this second crystal does not extend as far as that observed in the main subject crystal. Its more modest extension is perhaps, in turn, a reason why the peeling effect can cycle at least 3 times in the second crystal, while the main subject crystal was so tempered by the cyclical build-up of light-induced crystal strain lines that it had restored itself and fully halted any further peeling effect after two cycles of light and heat. Indeed, a fourth cycle of light-induction and warming on the main subject crystal was performed six months after the original three cycles of experiments, and the results were a replica of its cycle 3 (see Supplementary Information, Movie S7).
A complete interpretation of this phenomenon may not be as simple as considering straininduced tempering versus crystal peeling effects, though, since the extent of thermally-induced restorative effects of the crystal will also influence the ability of a crystal to undergo lightinduced crystal strain and peeling behavior. The second crystal continues to peel across three cycles, and appears to attempt to restore itself given the general reversal of the light-induced peeling upon warming. However, an underlayer of the second crystal slips significantly during the warming phase of cycle 1 (see Movie S4), which precludes the crystal from ever fully restoring itself; the physical mis-match in layers persists over cycles 2 and 3 and the crystal fractures in a few places during its pursuit to thermally recover. Despite the progressive deterioration of the crystal, it maintains its ability to peel over at least the 3 cycles studied, and the peeling effect appears to be essentially elastic in origin. Such origins of force can be compared with those from recent studies on elastic37 and plastic38 bending effects in crystals.
Thermal energy appears to compensate for the more modest light-induced peeling effect that is observed in the second crystal owing to its greater light-induced crystal strain. Thermal energy releases some of this crystal strain upon warming such that the initial warming phase of the second crystal actually raises the extent of peeling in the region 135 ± 10 K < T < 165 ± 10 K, whereupon it reaches its maximum peeling limit. It is noteworthy that the temperature onset of this further peeling corresponds to the temperature at which ƞ1-OSO photo-isomers observed in [Ru-SO2] complexes start to decay into a more thermally robust, metastable, side-bound ƞ2-SO2 configuration (T ~ 120-130 K).27,29 The crystal maintains this maximum extent of peeling upon further warming until about T = 215 ± 5 K where it starts to curl down as far as it can within the physical constraint that the frozen oil that holds the crystal on the sapphire substrate within the cryostat. This temperature aligns with the typical temperature range, T = 200-220 K,
whereby the side-bound ƞ2-SO2 isomer thermally decays back to its dark-state ƞ1-SO2 configuration. This physical ‘clamping’ effect is overcome once the oil melts at T = 230-240 ± 5 K, whereupon the peeling effect curls down fully as the crystal settles into a stationary state as it continues to warm to room temperature. These distinct warming phases are present in the light and warming cycles 1 and 2 for the main subject crystal but are much more subtle in their manifestation, cf, Movie S1 and Movie S2. The good and consistent match between these temperature-dependent curling effects and well-known temperature-dependent ƞ1-OSO ƞ2SO2 ƞ1-SO2 linkage isomer conversions in [Ru-SO2] complexes is particularly compelling evidence to corroborate the relationship between the macroscopic peeling effect in 1 and its nano-optical switching origins.
Overall, there is good reproducibility and consistency between the optical microscopy results for the two crystals studied, and where differences occur, these can be rationalized and offer further insights into the mechanistic behavior of the crystal peeling effect. One difference worth highlighting is that the aspect ratio of the crystal appears to affect the precise nature and extent of the crystal strain and peeling behavior of 1. An optical microscopy study of many crystals that span a large range of aspect ratios is needed in order to establish detailed relationships between the strain, peeling, thermal recovery and restorative characteristics of the crystal. A pre-requisite for such a study would be an extensive exploration of crystal growth mechanisms of 1 in order to furnish a set of new crystals that possess many different types of crystal habits with a large range of disparate aspect ratios for investigation. Establishing such relationships is beyond the scope of this work, but their projected realization could eventually enable the characteristics of this peeling effect to become tunable. This leads to the ultimate goal of tailoring these light-induced optical actuators to suit a given nano-optical switching application.
In summary, we have discovered a new material that undergoes a light-induced structural change in its single-crystal form, and demonstrated a relationship between its nano-optical switching effect and its macroscopic behavior to light. The field of single-crystal optical actuators is still in its infancy, but our showcasing of structure-function relationships in 1 across the molecular and macroscopic length scales stands to be transformative, in terms of showcasing to this field a means for creating crystalline materials with opto-mechanical function. This argument is especially pertinent when we consider the enormous prospects of these types of single-crystals as
The reaction precursor [Ru(NH3)4(SO2)Cl]Cl was synthesized according to literature methods.1 All other reagents were purchased from Sigma Aldrich and used without further purification.
[Ru(NH3)4(SO2)Cl]Cl (5 mg, 16 μmol) in an aqueous solution of Na2CO3 (200 μL, 1 M) which was mixed with another solution of 3-phenylpyridine (5 μL, 35 μmol) in methanol (200 μL). The resultant mixture immediately turned yellow. Subsequently, hydrochloric acid (100 μL, 32%) was added dropwise and orange crystals were formed within 1 h. Finally, the product was recovered by vacuum filtration and washed three times with methanol.
Dark and Photo-induced In Situ Single-Crystal X-ray Diffraction
The crystal structures of the dark- and light-induced states of 1 were determined using synchrotron-based X-ray crystallography, at the NSF’s ChemMatCARS beamline of the Advanced Photon Source, Argonne National Laboratory, IL, USA. A 0.120 × 0.030 × 0.005 mm3 single crystal of 1 was mounted onto a Huber three-circle diffractometer equipped with a Pilatus 3 x CdTe 1 M shutterless pixel array detector and a 100 K nitrogen open-flow cryostream
delivered by an Oxford cryojet. An X-ray beam of wavelength 0.41328 Å was used to capture a series of data frames over multiple ϕ scans of crystal orientations, collected in 0.3° increments each with 1.0 s exposure time, using five fixed (ω, κ) setups where the diffractometer sat at (−200°, 30°), (−190°, 20°), (−180°, 30°), (−180°, 15°), and (−180°, 0°) respectively, while maintaining a 130 mm sample-to-detector distance. For control purposes, the ambient lighting in the experimental hutch of the beamline was extinguished while data were being acquired for both dark- and light-induced crystal structure determinations. Data for the dark-state crystal structure were first obtained. The crystal was then maintained at 100 K on the diffractometer and rotated continuously while being irradiated with 505 nm light for 2.5 h, using a Thorlabs M505L3 lightemitting diode (LED) whose head power output was 1000 mA constant current and 3.3 V forward voltage. This light was switched off before acquiring data for the light-induced crystal structure. Further experimental details, as well as structure solution and refinement information, are given in the Supporting Information, S6−S9. A more detailed description of the specialized photocrystallography aspects of these experiments is given elsewhere.17-20
Single crystal optical characterization
A custom-built micro-spectroscopy system was used to record the absorption spectrum of single crystals under a variety of environmental conditions. The system was built around an inverted microscope (Olympus: IX71) coupled to a 300 mm focal length spectrograph (Princeton Instruments: Acton Series 2300i) and 1320 x 100 channel CCD camera (Princeton Instruments: PIXIS 100BR). A 0.190 x 0.070 x 0.010 mm3 crystal of 1 was mounted on a sapphire disk (9 mm dia., 0.5 mm thick) and fastened with a small amount of viscous perfluoroether oil. The mounted
sample was then placed on the cold finger of an optical cryostat (Janis: ST-500-UC) attached to the microscope. The cold finger was drilled through, allowing optical absorption measurements to be made. The crystal was positioned such that only half of the active vertical channels of the CCD camera were used to image a portion of the crystal using a 10 x, 0.13 NA objective (Olympus, NeoSPlan); the remaining half of the active detector channels imaged the sapphire substrate. The probe light for optical absorption measurements was provided by the microscope’s 100 W tungsten-halogen lamp and 0.3 NA condenser optics. A visible bandpass filter (Schott: BG40) and OD 9 neutral density filter was placed between the lamp and the condenser to reduce the thermal load on the sample and cryostat.
To induce photo-isomerization, the crystal was illuminated with 505 nm light from a ThorLabs M505F1 fiber optically coupled light-emitting diode (LED). The light from the LED was collimated and then coupled into the microscope through a side port, focusing it onto the back aperture of the objective, thus filling the field of view and evenly illuminating the entire crystal. The excitation power measured at the objective was typically 370 μW giving an estimated 340 μW illuminating the field of view.
Optical absorption spectra were recorded by imaging the crystal on the entrance slit (75 μm) of the spectrometer and dispersing the light, using a 150 line/mm grating, onto the detector. The image was positioned such that 30 rows of the detector were illuminated with light that passed through the crystal (IT); whereas 30 rows of the detector directly above the crystal recorded light that passed through only the sapphire substrate (I0). Absorption spectra were then calculated as -log10(IT/I0).
ASSOCIATED CONTENT Supporting Information. The following files are available free of charge. Movies (MOV) associated with Figure 2 and 3 showing the three cycles (Movies S1-3 respectively) of light-induced photo-isomerization process and thermal recovery of the main subject crystal to its dark state; analogous movies that demonstrate reproducibility of the peeling effect via a second crystal that undergoes three cycles of light-induction and warming (Movies S4-6); movie of the original crystal undergoing a fourth cycle of light-induction and warming 6 months after cycles 1-3 (Movie S7); Crystallographic Information Files (CIFs) for 1 in its darkand light-induced state; crystal structure refinement details, especially those associated with the twinning and disorder of 1 (PDF).
AUTHOR INFORMATION Corresponding Author * Email for correspondence: [email protected] Author Contributions J.M.C. performed all of the photocrystallography, optical microscopy, and absorption spectroscopy work, with experimental assistance from S.G.W and Y.-S.C. in beamline operation at the synchrotron and D.J.G. in setting up the optical microscopy and absorption spectroscopy apparatus. J.M.C. was the PhD supervisor of J.d.J.V. who synthesized the material. J.M.C. drafted the paper manuscript, which was written through contributions of all authors. All authors have given approval to the final version of the manuscript.
Notes The authors declare no competing financial interest.
ACKNOWLEDGMENTS J.M.C. thanks the 1851 Royal Commission of the Great Exhibition for the 2014 Fellowship in Design, hosted by Argonne National Laboratory where work done was supported by U.S. Department of Energy (DOE) Office of Science, Office of Basic Energy Sciences, and used research resources of the Center of Nanoscale Materials and the Advanced Photon Source (APS), Office of Science User Facilities operated for the DOE Office of Science by Argonne National Laboratory, supported by the U.S. DOE, all under contract No. DE-AC02- 06CH11357. Within the APS, NSF’s ChemMatCARS Sector 15 is principally supported by the Divisions of Chemistry (CHE) and Materials Research (DMR), National Science Foundation, under grant number NSF/CHE-1346572 and NSF/CHE-1834750. Use of the PILATUS3 X CdTe 1M detector is supported by the National Science Foundation under the grant number NSF/DMR1531283. J.M.C. is indebted to the BASF / Royal Academy of Engineering Senior Research Fellowship in Data-Driven Molecular Engineering of Functional Materials, and the ISIS Facility, STFC Rutherford Appleton Laboratory, UK, for financial support. J.d.J.V. acknowledges the National Council of Science and Technology of Mexico (CONACyT) and the Cambridge Trust for a PhD Scholarship (217553).
1. Abendroth, J. M.; Bushuyev, O. S.; Weiss, P. S.; Barrett, C. J. Controlling Motion at the Nanoscale: Rise of the Molecular Machines. ACS Nano 2015, 9, 7746–7768. 2. Midolo, L.; Schliesser, A.; Fiore, A. Nano-opto-electro-mechanical Systems. Nat. Nanotechnol. 2018, 13, 11-18. 3. Bochmann, J.; Vainsencher, A.; Awschalom, D. D.; Cleland, A. N. Nanomechanical Coupling between Microwave and Optical Photons. Nat. Phys. 2013, 9, 712-716. 4. Naumov, P.; Chizhik, S.; Panda, M. K.; Nath, N. K.; Boldyreva, E. Mechanically Responsive Molecular Crystals. Chem. Rev. 2015, 115, 12440-12490. 5. Zhu, L.; Al-Kaysi, R. O.; Bardeen, C. J. Photoinduced Ratchet-like Rotational Motion of Branched Molecular Crystals. Angew. Chem., Int. Ed. 2016, 55, 7073-7076. 6. Kim, K.; Al-Muhanna, M. K.; Al-Suwaidan, S. D.; Al-Kaysi, R. O.; Bardeen, C. J. Photoinduced Curling of Organic Molecular Crystal Nanowires. Angew. Chem. 2013, 125, 70277031 and Angew. Chem., Int. Ed. 2013, 27, 6889-6893. 7. Koshima, H.; Ojima, N.; Uchimoto, H. Mechanical Motion of Azobenzene Crystals upon Photoirradiation. J. Am. Chem. Soc. 2009, 131, 6890-6891. 8. Bushuyev, O. S.; Singleton, T. A.; Barrett, C. J. Fast, Reversible, and General Photomechanical Motion in Single Crystals of Various Azo Compounds using Visible Light. Adv. Mater. 2013, 25, 1796-1800.
9. Colombier, I.; Spagnoli, S.; Corval, A.; Baldeck, P. L.; Giraud, M.; Leaustic, A.; Yu, P.; Irie, M. Diarylethene Microcrystals make Directional Jumps upon Ultraviolet Irradiation, J. Chem. Phys. 2007, 126, 011101-011101. 10. Medishetty, R.; Husain, A.; Bai, Z.; Runcevski, T.; Dinnebier, R. E.; Naumov, P.; Vittal, J. J. Single Crystals Popping under UV light: the First Example of a Photosalient Effect Triggered by a [2+2] Cycloaddition Reaction. Angew. Chem., Int. Ed. 2014, 53, 5907-5911. 11. Natarajan, A.; Tsai, C. K.; Khan, S. I.; McCarren, P.; Garcia-Garibay, M. A. The Photoarrangement of -Santonin is a Single-crystal-to-single-crystal Reaction: a Long kept Secret in Solid-state Organic Chemistry Revealed. J. Am. Chem. Soc. 2007, 129, 9846-9847. 12. Tong, F.; Al-Haidar, M.; Zhu, L.; Al-Kaysi, R. O.; Bardeen, C. J. Photoinduced Peeling of Molecular Crystals. Chem. Commun. 2019, 55, 3709-3712. 13. Ashcroft, C. M.; Cole, J. M. Molecular Engineering of Organic and Organometallic Secondorder Nonlinear Optical Materials. In Handbook of Organic Materials for Electronic and Photonic Devices, 2nd Edition, Ostroverkhova, O., Ed.; Woodhead Publishing, Cambridge, 2019; p 152. 14. Coppens, P.; Novozhilova, I.; Kovalevsky, A. Photoinduced Linkage Isomers of Transitionmetal Nitrosyl Compounds and Related Complexes. Chem. Rev. 2002, 102, 861-884. 15. Masciocchi, N.; Kolyshev, A. N.; Dulepov, V. E.; Boldyreva, E. V.; Sironi, A. Study of the Linkage Isomerization [Co(NH3)5NO2]Br2 <=> [Co(NH3)5ONO]Br2 in the Solid State by X-ray Powder Diffraction. Inorg. Chem. 1994, 33, 2579-2585.
16. Naumov, P.; Sahoo, S. C.; Zakharov, B. A.; Boldyreva, E. V. Dynamic Single Crystals: Kinematic Analysis of Photoinduced Crystal Jumping (the Photosalient Effect). Angew. Chem., Int. Ed. 2013, 52, 9990-9995. 17. Coppens, P.; Fomitchev, D. V.; Carducci, M. D.; Culp, K. Crystallography of Molecular Excited States: Transition Metal Nitrosyl Complexes and the Study of Transient Species. Dalton Trans. 1998, 6, 865-872. 18. Cole, J. M. Single-crystal X-ray Diffraction Studies of Photo-induced Molecular Species. Chem. Soc. Rev. 2004, 33, 501-513. 19. Cole, J. M. Photocrystallography. Acta Crystallogr. A 2008, 64, 259-271. 20. Cole, J. M. A New Form of Analytical Chemistry: Distinguishing the Molecular Structure of Photo-induced States from Ground-states. Analyst 2011, 136, 448-455. 21. Kovalevsky, A. Y.; Bagley, K. A.; Coppens, P. The first Photocrystallographic Evidence for Light-induced Metastable Linkage Isomers of Ruthenium Sulfur Dioxide Complexes, J. Am. Chem. Soc. 2002, 124, 9241-9248. 22. Kovalevsky, A. Y.; Bagley, K. A.; Cole, J. M.; Coppens, P. Light-induced Metastable Linkage Isomers of Ruthenium Sulfur Dioxide Complexes. Inorg. Chem. 2003, 42, 140-147. 23. Bowes, K. F.; Cole, J. M.; Husheer, S. L. G.; Raithby, P. R.; Savarese, T. L.; Sparkes, H. A.; Teat, S. J.; Warren, J. E. Photocrystallographic Structure Determination of a new Geometric Isomer of [Ru(NH3)4(H2O)(η1-OSO)][MeC6H4SO3]2. Chem. Commun. 2006, 2448-2450.
24. Phillips, A. E.; Cole, J. M.; d’Almeida, T.; Low, K. S. Effects of the Reaction Cavity on Metastable Optical Excitation in Ruthenium-sulfur Dioxide Complexes. Phys. Rev. B 2010, 82, 155118. 25. Phillips, A. E.; Cole, J. M.; d’Almeida, T.; Low, K. S. Ru–OSO Coordination Photogenerated
Camphorsulfonate. Inorg. Chem. 2012, 51, 1204-1206. 26. Sylvester, S. O.; Cole, J. M.; Waddell, P. G. Photoconversion Bonding Mechanism in Ruthenium Sulfur Dioxide Linkage Photoisomers Revealed by In Situ Diffraction. J. Am. Chem. Soc. 2012, 134, 11860-11863. 27. Sylvester, S. O.; Cole, J. M. Solar-powered Nanomechanical Transduction from Crystalline Molecular Rotors. Adv. Mater. 2013, 25, 3324-3328. 28. Sylvester, S. O.; Cole, J. M. Quantifying Crystallographically Independent Optical Switching Dynamics in Ru SO2 Photoisomers via Lock-and-key Crystalline Environment. J. Phys. Chem. Lett. 2013, 4, 3221-3226. 29. Sylvester, S. O.; Cole, J. M.; Waddell, P. G.; Nowell, H.; Wilson, C. SO2 Phototriggered Crystalline Nanomechanical Transduction of Aromatic Rotors in Tosylates: Rationalization via Photocrystallography of [Ru(NH3)4SO2X]tosylate2 (X = pyridine, 3-Cl-pyridine, 4-Cl-pyridine). J. Phys. Chem. C 2014, 118, 16003–16010. 30. Chemicalize was used for prediction of pKa values, https://chemicalize.com/ accessed April 2019, developed by ChemAxon (http://www.chemaxon.com).
31. Jacobsen, R. S.; Andersen, K. N.; Borel, P. I.; Fage-Pedersen, J.; Frandsen, L. H.; Hansen, O.; Kristensen, M.; Lavrinenko, A. V.; Moulin, G.; Ou, H.; Peucheret, C.; Zsigri, B.; Bjarklev, A. Strained Silicon as a new Electro-optic Material. Nature 2006, 441, 199–202. 32. Pustogow, A.; McLeod, A. S.; Saito, Y.; Basov, D. N.; Dressel, M. Internal Strain Tunes Electronic Correlations on the Nanoscale. Sci. Adv. 2018, 4, eaau9123. 33. Lynch, S. M.; Shelbyy, J. Crystal Clamping in Lead Titanate Glass‐ Ceramics. J. Am. Ceram. Soc. 2006, 67, 424-427. 34. Liu, G.; Liu, J.; Ye, X.; Nie, L.; Gu, P.; Tao, X.; Zhang, Q. Self-Healing Behavior in a Thermo-Mechanically Responsive Cocrystal during a Reversible Phase Transition. Angew. Chem. Int. Ed. 2017, 56, 198-202. 35. Gupta, P.; Karothu, D. P.; Ahmed, E.; Naumov, P.; Nath, N. K. Thermally Twistable, Photobendable, Elastically Deformable, and Self-Healable Soft Crystals. Angew. Chem. Int. Ed. 2018, 57, 8498-8502. 36. Karothu, D. P.; Weston, J.; Desta, I. T.; Naumov, P. Shape-Memory and Self-Healing Effects in Mechanosalient Molecular Crystals. J. Am. Chem. Soc. 2016, 138, 13298-13306. 37. Worthy, A.; Grosjean, A.; Pfrunder, M. C.; Xu, Y.; Yan, C.; Edwards, G.; Clegg, J. K.; McMurtrie, J. C. Atomic Resolution of Structural Changes in Elastic Crystals of Copper(II) Acetylacetonate. Nat. Chem. 2018, 10, 65-69. 38. Panda, M. K.; Ghosh, S.; Yasuda, N.; Moriwaki, T.; Mukherjee, G. D.; Reddy, C. M.; Naumov, P. Spatially Resolved Analysis of Short-Range Structure Perturbations in a Plastically Bent Molecular Crystal. Nat. Chem. 2015, 7, 65-72.